Low-temperature synthesis of LiFePO4 nanocrystals by solvothermal route
© Lim et al; licensee Springer. 2012
Received: 20 September 2011
Accepted: 5 January 2012
Published: 5 January 2012
LiFePO4 nanocrystals were synthesized at a very low temperature of 170°C using carbon nanoparticles by a solvothermal process in a polyol medium, namely diethylene glycol without any heat treatment as a post procedure. The powder X-ray diffraction pattern of the LiFePO4 was indexed well to a pure orthorhombic system of olivine structure (space group: Pnma) with no undesirable impurities. The LiFePO4 nanocrystals synthesized at low temperature exhibited mono-dispersed and carbon-mixed plate-type LiFePO4 nanoparticles with average length, width, and thickness of approximately 100 to 300 nm, 100 to 200 nm, and 50 nm, respectively. It also appeared to reveal considerably enhanced electrochemical properties when compared to those of pristine LiFePO4. These observed results clearly indicate the effect of carbon in improving the reactivity and synthesis of LiFePO4 nanoparticles at a significantly lower temperature.
The orthorhombic olivine structure of LiFePO4 is intensively investigated as the most attractive cathode to replace commercialized LiCoO2 in rechargeable lithium-ion batteries because it is not only inexpensive, nontoxic, and environmentally benign, but has also a relatively high theoretical capacity of 170 mAh g-1 and a suitably flat voltage region of 3.45 V within the electrolyte window . However, despite these advantages, its unimpressive rate performance due to intrinsic problems of low ionic and electronic conductivities still remains as a major obstacle for commercial applications. Progressive efforts to circumvent this obstacle by carbon coating on particle surface , developing composites via mixing conductive materials , aliovalent cation substitution , particle size minimization [5, 6], and customizing particle morphologies [7–11] have been undertaken.
Among these approaches, with respect to Li-ion batteries, nano-sized electrodes have been intensively investigated for high-power density applications as the advantage of using such electrodes remains twofold [12, 13]. Firstly, nanomaterials provide a favorable structural framework that ensures shorter diffusion paths for the Li-ions to traverse from the core of the particles to the surface through the lattice, thereby yielding excellent electrochemical properties. Secondly, the large surface area of nanomaterials ensures enhanced electrode/electrolyte interfacial contact, thus leading to higher charge/discharge rates and good capacity retentions [14, 15]. In addition, it is also evident that customizing particle morphologies is becoming highly important since these factors are well known to significantly influence material properties and electrochemical performances.
Ultimately, designing nanomaterials is a critical issue for the industrial applications because device performance is hugely dependent on material properties. In addition, the efficacy of technologies for nanomaterials largely depends on preparation and processing methods. To date, various synthesis techniques have been adopted for synthesizing nano-sized LiFePO4 and controlling the morphology of LiFePO4 nanoparticles by soft chemistry processes such as co-precipitation , sol-gel , hydrothermal [7, 8, 18], polyol [11, 15], and solvothermal methods [9, 10, 19, 20]. Our group has introduced inexpensive and simple processes of conventional polyol method, microwave-assisted polyol process and solvothermal method using the polyol media, which are new methods of synthesizing LiFePO4 with well-defined nanoparticles and high crystallinity, without the need for any further heating as a post-treatment [15, 19, 21, 22]. In these processes, the polyol media play an important role not only as solvents, but also as a reducing environmental agent and stabilizer, thereby limiting particle growth and preventing agglomeration . Among these processes, the solvothermal process is especially advantageous for synthesizing LiFePO4, which can obtain nanoparticles with high crystallinity at a relatively low temperature because of high pressure at a moderate temperature, compared with conventional and microwave-assisted polyol process. Also, we have reported that nano-sized LiMPO4(M = Fe, Mn, Co) has been synthesized at a reaction temperature of 200°C by solvothermal method in which the LiFePO4 sample has showed good electrochemical properties [19, 20, 23]. When we have used various polyol media of ethylene glycol [EG], diethylene glycol [DEG], triethylene glycol [TEG], and tetraethylene glycol [TTEG] for synthesizing LiFePO4 nanoparticles at a temperature of 200°C, it was confirmed that reactivity might be affected because a pressure in the bomb during the solvothermal reaction is different according to the boiling point of the polyol media .
In this work, we report synthesizing nanostructured LiFePO4 with an olivine structure and high crystallinity by solvothermal method employing carbon nanoparticles at a very low temperature of 170°C. The physical properties and electrochemical performances of the obtained LiFePO4 samples were investigated.
LiFePO4 without carbon
LiFePO4 was synthesized by solvothermal process as follows: (C2H3O2)2Fe (99.995%; Sigma-Aldrich, Yongin-city, Kyunggi-do, South Korea), H3PO4 (above 85%; Daejung Chemicals & Metals Co., Ltd, Shiheung-city, Gyeonggi-Do, South Korea), and CH3COOLi·2H2O (GR, Junsei Chemical Co., Ltd, Tokyo, Japan) were added to (HOCH2CH2)2O (99%; Daejung Chemicals & Metals Co., Ltd) in the molar ratio 1:1:1 (Li:Fe:P) and stirred for about 30 min at room temperature. The mixed solution was transferred into a Teflon-lined bomb with a volume of 40 ml. The bomb was sealed and heated at mild temperatures for 16 h in a high-temperature conventional oven.
CH3COOLi·2H2O (GR, Junsei Chemical Co., Ltd), (C2H3O2)2Fe (99.995%, Sigma-Aldrich), H3PO4 (above 85%; Daejung Chemicals & Metals Co., Ltd), and diethylene glycol (99%; Daejung Chemicals) were used as the starting materials, and Ketjen Black was used as a carbon source. Initially, 10 wt% Ketjen Black was added in a 25-ml DEG solvent and treated with ultrasonic for 1 h. Subsequently, Fe, Li, and P precursors were added to the solution and stirred for 30 min at room temperature. The mixed solution was transferred into a Teflon-lined bomb with a volume of 40 ml. The bomb was sealed and heated at 170°C for 16 h in a high-temperature conventional oven.
After the solvothermal reaction, the resulting solutions containing grayish precipitates were washed with acetone and methanol several times in order to ensure removal of the organic compounds, respectively. The obtained precipitates were separated by filtering using ceramic membrane funnels and dried at 120°C for 12 h in a vacuum oven.
Structural and physical characterization
Powder X-ray diffraction [XRD] data of the obtained samples were recorded using a Shimadzu X-ray diffractometer with Ni-filtered Cu Kα radiation (λ = 1.5406 Å) operating at 40 kV and 30 mA within the scanning angle of 2θ, range 15° to 60° in steps of 0.02°. The particle morphologies and sizes were determined by field emission-scanning electron microscopy [FE-SEM].
The electrochemical properties of the LiFePO4 samples were evaluated with lithium metal as the reference and counter electrode. For the electrochemical measurements, the active material was mixed with conductive carbon (Ketjen Black), and Teflonized Acethylene Black was used as a binder. The mixture was pressed onto a stainless steel mesh and vacuum dried at 120°C for 12 h, thus forming the cathode. A 2032 coin-type cell consisting of the cathode and lithium metal anode separated by a polymer membrane together with glass fiber was fabricated in an Ar-filled glove box and aged for 12 h before the electrochemical measurements. The electrolyte employed was a 1:1 mixture of ethylene carbonate and dimethyl carbonate containing 1 M LiPF6.
Results and discussion
In our earlier paper, we showed that a pressure in the bomb during the solvothermal reaction at the same temperature might differ according to the polyol media of EG, DEG, TEG, and TTEG . Notably, among these polyol media, DEG was the most suitable for synthesizing the LiFePO4 nanoparticles at the same reaction temperature of 200°C due to the appropriate boiling point of 240°C. In terms of economics, lowering reaction temperature during synthesizing is one of the critical points in commercialization. Therefore, we have tried to lower the reaction temperature during solvothermal process using carbon and simultaneously obtain the olivine nanoparticles with high crystallinity.
LiFePO4 nanocrystals with high crystallinity were synthesized at a very low temperature of 170°C using carbon nanoparticles by a solvothermal process in a polyol medium, namely DEG without any heat treatment as a post procedure. In XRD pattern, all the peaks are indexed on the basis of an orthorhombic olivine-type structure (space group: Pnma), and no second phase such as Li3PO4 or transition metal compounds was observed though the sample without carbon revealed little impurity peaks. The LiFePO4 nanocrystals synthesized at low temperature exhibited mono-dispersed and carbon-mixed plate-type LiFePO4 nanoparticles with average length, width, and thickness of approximately 100 to 300 nm, 100 to 200 nm, and 50 nm, respectively. In order to certify better rate capability caused by particle size minimization and carbon effect in the LiFePO4 nanoparticles, galvanostatic test was performed using the carbon-mixed LiFePO4 and pristine LiFePO4 without carbon for comparison purposes. Further, the carbon-mixed LiFePO4 sample appeared to reveal considerably enhanced electrochemical properties when compared to those of pristine LiFePO4. Thus, the observed results clearly indicate the effect of carbon in improving the reactivity and significantly low-temperature synthesis of LiFePO4 nanoparticles.
This research was supported by the Ministry of Knowledge Economy, Korea, under the Information Technology Research Center support program supervised by the National IT Industry Promotion Agency (NIPA-2012-C1090-1200-0002).
- Padhi AK, Nanjundaswamy KS, Goodenough JB: Phospho-olivines as positive-electrode materials for rechargeable lithium batteries. J Electrochem Soc 1997, 144: 1188. 10.1149/1.1837571View ArticleGoogle Scholar
- Ravert N, Chouinard Y, Magnan JF, Besner S, Gauthier M, Armand M: Electroactivity of natural and synthetic triphylite. Power Sources 2001, 97–98: 503.View ArticleGoogle Scholar
- Huang H, Yin S-C, Nazar LF: Approaching theoretical capacity of LiFePO4at room temperature at high rates. Electrochem Solid-State Lett 2001, 4: A170. 10.1149/1.1396695View ArticleGoogle Scholar
- Chung SY, Bloking JT, Chiang YM: Electronically conductive phosphor-olivines as lithium storage electrodes. Nat Mater 2002, 1: 123. 10.1038/nmat732View ArticleGoogle Scholar
- Yamada A, Nishimura S, Koizumi H, Kanno R, Seki S, Kobayashi Y, Miyashiro H, Dodd J, Yazami R, Fultz B: Intermediate phases in LixFePO4. Mater Res Soc Symp Proc 2007, 972-AA13–02: 257.Google Scholar
- Delacourt C, Poizot P, Levasseur S, Masquelier C: Size effects on carbon-free LiFePO4powders. Electrochem Solid-State Lett 2006, 9: A352. 10.1149/1.2201987View ArticleGoogle Scholar
- Dokko K, Koizumi S, Nakano H, Kanamura K: Particle morphology, crystal orientation, and electrochemical reactivity of LiFePO4synthesized by the hydrothermal method at 443 K. J Mater Chem 2007, 17: 4803. 10.1039/b711521kView ArticleGoogle Scholar
- Ellis B, Kan WH, Makahnouk WRM, Nazar LF: Synthesis of nanocrystals and morphology control of hydrothermally prepared LiFePO4. J Mater Chem 2007, 17: 3248. 10.1039/b705443mView ArticleGoogle Scholar
- Murugan AV, Muraliganth T, Manthiram A: Rapid microwave-solvothermal synthesis of phospho-olivine nanorods and their coating with a mixed conducting polymer for lithium ion batteries. Electrochem Commun 2008, 10: 903. 10.1016/j.elecom.2008.04.004View ArticleGoogle Scholar
- Saravanan K, Balaya P, Reddy MV, Chowdari BVR, Vittal JJ: Storage performance of LiFePO4nanoplates. J Mater Chem 2008, 19: 605.View ArticleGoogle Scholar
- Kim D, Lim J, Choi E, Gim J, Mathew V, Paik Y, Jung H, Lee W, Ahn D, Paek SM, Kim J: Synthesis of highly crystalline olivine-type LiFePo4nanoparticles by solution-based reactions. Surface Review and Letters 2010, 17: 111. 10.1142/S0218625X10014053View ArticleGoogle Scholar
- Alivisatos AP: Semiconductor clusters, nanocrystals, and quantum dots. Science 1996, 271: 933. 10.1126/science.271.5251.933View ArticleGoogle Scholar
- Kim J, Manthiram A: Amanganese oxyiodide cathode for rechargeable lithium batteries. Nature 1997, 390: 265. 10.1038/36812View ArticleGoogle Scholar
- Kim DH, Ahn YS, Kim J: Polyol-mediated synthesis of Li4Ti5O12nanoparticle and its electrochemical properties. Electrochem Commun 2005, 7: 1340. 10.1016/j.elecom.2005.09.027View ArticleGoogle Scholar
- Kim DH, Kim J: Synthesis of LiFePO4nanoparticles in polyol medium and their electrochemical properties. Electrochem Solid-State Lett 2006, 9: A439. 10.1149/1.2218308View ArticleGoogle Scholar
- Arnold G, Garche J, Hemmer R, Strobele S, Volger C, Wohlffahrt-Mehrens M: Fine-particle lithium iron phosphate LiFePO4synthesized by a new low-cost aqueous precipitation technique. J Power Sources 2003, 119–121: 247.View ArticleGoogle Scholar
- Yang J, Xu JJ: Nonaqueous sol-gel synthesis of high-performance LiFePO4. Electrochem Solid-State Lett 2004, 7: A515. 10.1149/1.1819893View ArticleGoogle Scholar
- Yang S, Zavalij P, Whittingham MS: Hydrothermal synthesis of lithium iron phosphate cathodes. Electrochem Commun 2001, 3: 505. 10.1016/S1388-2481(01)00200-4View ArticleGoogle Scholar
- Lim JS, Kim DH, Jung IO, Woo CH, Choi ES, Gim JH, Kim J: Synthesis and electrochemical properties of LiMPO4(M = Fe, Mn, Co) nanocrystals in polyol medium. J Nanosci Nanotech 2010, 10: 3357. 10.1166/jnn.2010.2311View ArticleGoogle Scholar
- Lim J, Kim D, Mathew V, Kim J: Synthesis of LiMPO4(M = Fe, Mn, Co) nanocrystals in polyol medium and their electrochemical properties. Phys Scr 2010, T139: 014060.View ArticleGoogle Scholar
- Kim DH, Im JS, Kang JW, Kim EJ, Ahn HY, Kim J: A new synthesis route to nanocrystalline olivine phosphates and their electrochemical properties. J Nanosci Nanotech 2007, 7: 3949. 10.1166/jnn.2007.102View ArticleGoogle Scholar
- Kim DH, Kang JW, Jung IO, Im JS, Kim EJ, Song SJ, Lee JS, Kim J: Microwave assisted synthesis of nanocrystalline Fe-phosphates electrode materials and their electrochemical properties. J Nanosci Nanotech 2008, 8: 5376. 10.1166/jnn.2008.1388View ArticleGoogle Scholar
- Lim J, Kim D, Mathew V, Ahn D, Kang J, Kang SW, Kim J: Plate-type LiFePO4nanocrystals by low temperature polyol-assisted solvothermal reaction and its electrochemical properties. J Alloys and Compounds 2011, 509: 8130. 10.1016/j.jallcom.2011.05.081View ArticleGoogle Scholar
- Lim J, Kim D, Mathew V, Ahn D, Kim J: Synthesis of LiFePO4nanoparticles by solvothermal process using various polyol media and their electrochemical properties. J Nanosci Nanotech 2011, 11: 1451. 10.1166/jnn.2011.3342View ArticleGoogle Scholar
- Choi ES, Kim DH, Woo CH, Choi CH, Kim J: Synthesis and electrochemical properties of LiFePO4/carbon nanocomposites in polyol medium. J Nanosci Nanotech 2010, 10: 3416. 10.1166/jnn.2010.2310View ArticleGoogle Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.